Using MATLAB to Design and Analyse Composite Laminates


 Anissa Simmons
 1 years ago
 Views:
Transcription
1 Engineering, 2010, 2, doi: /eng Published Online November 2010 ( Using MATLAB to Design and Analyse Composite Laminates Abstract Avinash Ramsaroop, Krishnan Kanny * Department of Mechanical Engineering, Durban University of Technology, Durban, South Africa Received July 3, 2010; revised August 5, 2010; accepted August 19, 2010 This work deals with the generation of MATLAB script files that assists the user in the design of a composite laminate to operate within safe conditions. The inputs of the program are the material properties, material limits and loading conditions. Equations based on Hooke s Law for twodimensional composites were used to determine the global and local stresses and strains on each layer. Failure analysis of the structure was performed via the TsaiWu failure theory. The output of the program is the optimal number of fibre layers required for the composite laminate, as well as the orientation of each layer. Keywords: Composite Laminates, Hooke s Law, Fibre Angle, MATLAB, Composite Design 1. Introduction Composites are etremely versatile materials and may be tailored to suit any function. They have found uses from the aerospace industry to common everyday applications. However, one drawback of these materials is tedious design processes [1]. Therefore, in an attempt to reduce this time consuming phase, it was decided to develop a computer program that assisted the user in designing a composite structure. The program needed to perform the necessary calculations in the fraction of the time it would take if done using conventional techniques. Conventional methods for designing composite structures involve the use of Hooke s law for twodimensional unidirectional composites. Equations relating the stresses and strains in these materials have been developed and are available from various tets [24]. These equations, however, are limited to flat unidirectional laminates. The procedure to follow is quite laborious. The material properties, material limits, number of fibre layers, and the fibre orientation and thickness of each layer as well as the loading conditions need to be known. These quantities are then used in the governing equations and numerous matri computations are required. The outputs from these equations are the global and local stresses and strains of each layer. The local stresses on each layer are then compared to the allowable material limits and, if they eceed these limits, the entire process needs to be repeated with new angles and, if necessary, more fibre layers. If a composite structure has to be designed to optimally carry the applied loads, the manual calculations would take an etremely long time. Designers usually use standard fibre angles in their design to overcome the time factor because eact fibre orientation is diffic [5]. As a res composite structures are usually overdesigned as incorrect fibre angles may mean more fibre layers which in turn leads to increased material costs. Many researchers [69] have attempted to reduce material costs by reducing the laminate thickness but these were based on fied fibre angles. Certain regions of a composite structure, such as holes and other high stress zones, may need more reinforcement than others. Only these areas would require more fibre layers. However, with the conventional approach to design, the entire structure would be laid up to compensate for the high stress concentrations which increases the material costs. Therefore an approach was needed where the calculations can be performed easily and automatically, and where only the regions with high stresses have etra reinforcement. A logical solution was to write computer programs to perform the computations. MATLAB, a numerical computing package, was used as a basis for the programs as it is more than sufficient to handle the numerous matri computations [1014]. It may also be interfaced with programs written in other languages, such as C, C++, and FORTRAN [1314]. Basically, two programs were generated and each program consisted of a main script file and various functions. The first program was written according to the conventional methods for designing composite structures. The purpose of this program was to determine whether its
2 A. RAMSAROOP ET AL. 905 functions operated efficiently and performed calculations correctly as these would be used for the second program. Ress from this program were compared to manually calculated eamples. The second program used a different approach where the number of inputs were reduced to just the material properties, material limits and applied loading conditions. The outputs of this program are the number of layers and the fibre angle of each layer. These programs are discussed in further detail after the equations governing the stressstrain relationships are eamined. 2. Hooke s Law for TwoDimensional Composite Structures Figure 1 shows a schematic representation of a composite lamina. The direction along the fibre ais is designated 1. The direction transverse to the fibre ais but in the plane of the lamina is designated 2. The direction transverse to both the fibre ais and the plane of the lamina (out of page) is designated 3. This direction is not shown in the figure as it only becomes necessary in threedimensional cases. The 12 coordinate system can be considered to be local coordinates based on the fibre direction. However this system is inadequate as fibres can be placed at various angles with respect to each other and the structure. Therefore a new coordinate system needs to be defined that takes into account the angle the fibre makes with its surroundings. This new system is referred to as global coordinates (y system) and is related to the local coordinates (12 system) by the angle θ. A composite material is not isotropic and therefore its stresses and strains cannot be related by the simple Hooke s Law ( E ). This law has to be etended to twodimensions and redefined for the local and global coordinate systems [2]. The res is Equations (1) and (2). Figure 1. Global coordinate system in relation to local coordinate system. Q Q Q12 Q Q Q11 Q12 Q 16 y Q12 Q22 Q26 y y Q16 Q26 Q 66 y where σ 1,2 are the normal stresses in directions 1 and 2; τ 12 is the shear stress in the 12 plane; ε 1,2 are the normal strains in directions 1 and 2; γ 12 is the shear strain in the 12 plane; [Q] is the reduced stiffness matri; σ,y are the normal stresses in directions and y; τ y is the shear stress in the y plane; ε,y are the normal strains in directions and y; γ y is the shear strain in the y plane; [ Q ] is the transformed reduced stiffness matri. The elements of the [Q] matri in Equation (1) are dependent on the material constants and may be calculated using Equation (3). E E E Q, Q, Q, Q G (1) (2) (3) where E 1,2 are Young s modulus in directions 1 and 2; G 12 is the shear modulus in the 12 plane; ν 12,21 are Poisson s ratios in the 12 and 21 planes. The [ Q ] matri in Equation (2) may be determined by Equation (4). 1 1 Q T QRTR (4) where [T] is the transformation matri; [R] is the Reuter matri. These matrices are given by: 2 2 c s 2sc T s c 2sc and R (5) 2 2 sc sc c s where c = cosθ; s = sinθ. The local stresses and strains in Equation (1) are related to the global stresses and strains in Equation (2) by Equation (6) y T 2 and 2 RTR y y y Equations (1) to (6) are used to determine the stresses and strains for a single composite layer. Since composites are milayered entities, equations for this case must also be set up. The res is Equation (7). 0 N A B M B D (7) (6)
3 906 A. RAMSAROOP ET AL. where N is the vector of resant forces; M is the vector of resant moments; ε 0 is the vector of the midplane strains; κ is the vector of midplane curvatures. Vectors ε and κ are related to the global coordinates by Equation (8). 0 0 y y z y (8) 0 y y y where z is an arbitrary distance from the midplane. The [A], [B], and [D] matrices in Equation (7) are known as the etensional, coupling, and bending stiffness matrices, respectively. The elements of these matrices may be determined from Equations (9) to (11). n 1 A Q h h i 1, 2, 3 j 1, 2, 3 (9) ij ij k k k 1 k n 1 B Q h h i 1, 2, 3 j 1, 2, 3 (10) ij ij k k 2 k 1 k n 1 Dij Qij hk hk i 1, 2, 3 j 1, 2, 3 (11) 3 k 1 k where n is the number of layers; Qij is the ith, k jth element of the [ Q ] matri of the kth layer; h k is the distance of the top or bottom of the kth layer from the midplane of the composite. Figure 2 illustrates how to determine the distance h k from the midplane. The final aspect involved in the design of a composite structure is the failure analysis. There are various failure theories; however, the TsaiWu failure criterion is only one that closely correlates with eperimental data. This failure theory is given by Equation (12). H H H H H H 2H (12) The parameters for the TsaiWu failure criterion are given by Equation (13) H1 ; H2 ; H6 0 T C T C H11 ; H22 ; H66 T C T C H12 T C T C (13) T where 12, are the imate tensile stresses in direction 1 and 2; 12, are the imate compressive C stresses in direction 1 and 2; 12 is the imate shear stress in the 12 plane. In order to better facilitate the use of this failure theory, each stress component of Equation (12) was miplied by a variable [2]. This variable is referred to as the strength ratio (SR) and combining this in Equation (12) resed in Equation (14). ( H11 H22 H612) SR (14) ( H111 H222 H H1212 ) SR 1 The purpose of SR is to directly determine by what ratio the local stresses must be increased or decreased to avoid failure. This also directly relates to the applied forces. The criterion for SR is that it can only be positive. If SR is less than 1, then failure occurs because it means that the loading needs to decrease to avoid failure. A SR value of 1 implies that the composite structure is perfectly suited for the applied loading conditions. A value of greater than 1 means that the structure is more than capable of carrying the applied loading and that the loading may also be increased. For eample, a SR value of 1.5 means that the loading may be increased up to 50% without failure occurring. Figure 2. Locations of layers in a composite structure [2].
4 A. RAMSAROOP ET AL Programming 3.1. Conventional Approach Program This approach follows the commonly found methods laid out in the various tets [24]. As stated above, the material constants, material limits, number of fibre layers, fibre angle of each layer, and the thickness of each layer as well as the loading conditions need to be known. The following procedure illustrates the steps involved in this approach: 1) Calculate the [Q] matri for each layer using Equation (3). 2) Using Equation (5), compute the [T] matri for each layer. 3) Determine [ Q ] matri for each layer via Equation (4). 4) Find the location of the top and bottom surface of each layer, h k (k = 1 to n). 5) Use Equations (9), (10) and (11) to calculate the [A], [B], and [D] matrices. 6) Substitute these matrices as well as the applied loading into Equation (7) and solve the si simaneous equations to determine the midplane strains (ε 0 ) and curvatures (κ). 7) Find the global strains and stresses in each layer using Equations (8) and (2), respectively. 8) Find the local strains and stresses for each layer by using Equation (6). 9) Determine the parameters for the TsaiWu failure criterion via Equation (13). 10) Using these parameters and the local stresses for each layer, find SR via Equation (14). Once SR has been determined, the designer will know whether the structure will fail or not. If failure occurs, the fibre angles and possibly the number of layers have to be adjusted, and the above procedure needs to be repeated until no failure takes place. Manual calculations would take a long period, therefore a program was written to perform the necessary calculations. The program prompts the user for the following inputs: the material properties (E 1, E 2, G 12 and ν 12 ) the material limits ( T 1, C 1, T 2, C 2, 12 ) the number of layers (N) the fibre angle (θ) of each layer the thickness (t) of each layer applied loading conditions These input parameters were used to determine the [Q], [T], and [ Q ] matrices for each layer. All data concerning each layer (E 1, E 2, G 12, ν 12, θ, t, [Q], [T], and [ Q ]) were stored in an array. The data in this array was used to calculate the [A], [B], and [D] matrices. Using these matrices and the applied loading conditions, the global and local stresses and strains were computed. The local stresses were compared to the material limits, via the TsaiWu failure criterion, to determine whether the composite will fail. The computation of the various matrices and other relevant data was each carried out in a separate function. This means there was one function to determine the [Q] matri, another to calculate the [T] matri, and so on. A script file was written that controlled the use of each function. The purpose of the functions was to enable easier programming in future. This program was tested against manually calculated eamples in the various tets [2,3] and the ress were eactly comparable to the manual computations. In an eample (Eample 4.3) by Kaw [2], the stresses and strains in a graphite/epoy composite laminate were eamined. This laminate consisted of three layers, with fibre angles of 0, 30 and 45, and each layer had a thickness of 5 mm. The material properties, material limits and loading conditions used in this eample are given in Table 1. The resing global strains, global stresses, local strains and local stresses at the top, middle and bottom of each layer are shown in Figures 3 to 6, respectively. The values in Table 1 and the fibre angles of 0, 30 and 45 were used as inputs in the Conventional Approach script file. The global and local stresses and strains were computed and are shown in Figures 7 to 10. The values in these tables and the ones in Figures 3 to 6 are eactly comparable. The conclusion from this is that the Conventional Approach program can accurately determine the stresses and strains in a flat unidirectional composite structure. The Conventional Approach script file was further etended to include failure analysis via the TsaiWu failure theory. The resing SR values for the top, middle and bottom of each layer is shown in Figure 11. The rows represent the layers and columns 1 to 3 represent the top, middle and bottom of each layer, respectively. The SR values in Figure 11 indicate that the composite structure will fail first on layer 1 (SR = ) and then layer 2 (SR = ). It is clear from this that the input angles and number of layers were insufficient to carry the applied loads. Although this program performs all the relevant calculations easily and automatically, and significantly shortens the design process, using the program to design a composite structure would require much guesswork. The designer would enter the necessary input values, allow the program to perform the various calculations, and then discover whether the composite structure would fail. If failure does occur, as in the above case, the designer may have to change the fibre angles and/or the
5 908 A. RAMSAROOP ET AL. thickness of each layer and/or the number of layers. The choice of values may be uncertain and values would have to be assumed. Furthermore, it would also be an uncertainty on which values to change. Much time may be spent in achieving a structure that would not fail. On the other hand, if failure does not occur, the structure may prove to be overdesigned in which case the manufacturing costs of the structure may increase as unnecessary material will be used. To overcome these problems, a new script file was generated. Table 1. Material properties, limits and loading conditions for graphite/epoy composite eample in Kaw [2]. Material Properties Material Limits Forces Moments T C T C E 1 E 2 G ν (GPa) (GPa) (GPa) 12 (MPa) (MPa) (MPa) (MPa) (MPa) N M Table 4.1 Global Strains (m/m) in Eample 4.3 Ply # Position ε ε y γ y Top (10 8 ) (10 6 ) (10 6 ) 1 (0 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 6 ) Top (10 7 ) (10 6 ) (10 6 ) 2 (30 o ) Middle (10 7 ) (10 6 ) (10 7 ) Bottom (10 7 ) (10 6 ) (10 7 ) Top (10 7 ) (10 6 ) (10 7 ) 3 ( 45 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 6 ) Figure 3. Table from eample in Kaw [2] showing global strains. Table 4.2 Global Stresses (Pa) in Eample 4.3 Ply # Position y y Top (10 4 ) (10 4 ) (10 4 ) 1 (0 o ) Middle (10 4 ) (10 4 ) (10 4 ) Bottom (10 4 ) (10 4 ) (10 4 ) Top (10 4 ) (10 4 ) (10 4 ) 2 (30 o ) Middle (10 5 ) (10 4 ) (10 4 ) Bottom (10 5 ) (10 4 ) (10 4 ) Top (10 5 ) (10 5 ) (10 5 ) 3 ( 45 o ) Middle (10 4 ) (10 4 ) (10 4 ) Bottom (10 4 ) (10 4 ) (10 4 ) Figure 4. Table from eample in Kaw [2] showing global stresses. Table 4.3 Local Strains (m/m) in Eample 4.3 Ply # Position Top (10 8 ) (10 6 ) (10 6 ) 1 (0 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 6 ) Top (10 7 ) (10 6 ) (10 6 ) 2 (30 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 6 ) (10 6 ) (10 6 ) Top (10 6 ) (10 6 ) (10 6 ) 3 ( 45 o ) Middle (10 7 ) (10 6 ) (10 6 ) Bottom (10 7 ) (10 6 ) (10 7 ) Figure 5. Table from eample in Kaw [2] showing local strains.
6 A. RAMSAROOP ET AL. 909 Table 4.4 Local Stresses (Pa) in Eample 4.3 Ply # Position Top (10 4 ) (10 4 ) (10 4 ) 1 (0 o ) Middle (10 4 ) (10 4 ) (10 4 ) Bottom (10 4 ) (10 4 ) (10 4 ) Top (10 4 ) (10 4 ) (10 4 ) 2 (30 o ) Middle (10 5 ) (10 4 ) (10 4 ) Bottom (10 5 ) (10 4 ) (10 4 ) Top (10 5 ) (10 4 ) (10 4 ) 3 ( 45 o ) Middle (10 4 ) (10 4 ) (10 3 ) Bottom (10 4 ) (10 4 ) (10 3 ) Figure 6. Table from eample in Kaw [2] showing local stresses. Figure 7. Global strains from Conventional Approach program with Table 1 as inputs. Figure 8. Global stresses from Conventional Approach program with Table 1 as inputs.
7 910 A. RAMSAROOP ET AL. Figure 9. Local strains from Conventional Approach program with Table 1 as inputs. Figure 10. Local stresses from Conventional Approach program with Table 1 as inputs FibreAngleOutput Program Initially it was decided that this program should take the applied loading conditions, material properties and material limits as inputs. The program was to assume that the number of layers equals the number of input forces, and that the fibre angle of each layer equals the direction of each force. It would then perform all the necessary matri calculations as in the Conventional Approach. The global and local stresses and strains would be determined as before and failure analysis with the TsaiWu criterion may be performed. However, the assumptions made above cannot be used in a real situation as it may res in an overdesign of a composite structure as in the case of the conventional approach. Hence a program was written that does not make any assumptions but rather builds the laminate up one layer at a time. Basically this program varies the fibre angles to achieve a composite structure that is perfectly suited to carry the applied loading conditions. The
8 A. RAMSAROOP ET AL. 911 Figure 11. SR ratios from Conventional Approach program with Table 1 as inputs. outputs of the program are the number of layers and the fibre angle of each layer. The program asks the user to input the following: material properties material limits loading conditions The [Q] matri and the TsaiWu parameters can be calculated immediately as these do not vary with fibre angle but rather with material properties and limits. The program begins with one layer at an angle of 0 and computes h k, as well as the [T], [ Q ], [A], [B] and [D] matrices. Thereafter the midplane strains and curvatures, and, the global and local stresses and strains are calculated. The TsaiWu failure theory is applied and a value for SR is obtained for each layer. The program then analyzes the SR values and confirms whether it is in a certain range. The lower limit of this range is 1 as any value below this would mean failure. The upper limit in this range is 1.2 and this is to avoid overdesigning. If the SR value for each layer is between 1 and 1.2, then the design of the composite structure is complete. On the other hand, if the SR value for any of the layers is out of this range, the program varies that particular fibre angle to obtain a SR value between 1 and 1.2. However, due to the angle change all the matri calculations have to be redone. A new SR value is obtained for each layer and this is compared to the old values. If the new SR value for a particular layer is higher than the old SR value, then the angle of that layer is changed to the new one. For eample, after the initial calculation a layer with fibre angle of 30 has a SR value of 0.8. This is not acceptable and the program changes the angle to obtain a better SR value. Say at 35 the SR value is 0.9, the program will then change the angle of the 30 layer to 35. If at 35 the SR value was 0.7, then the program will retain the 30 angle. The program continues to change angles and compare old and new SR values until the SR value of each layer is between 1 and 1.2, in which case the design is completed. However, if this range cannot be achieved, a new layer is added on. The program starts from the beginning and recalculates the various matrices. SR values are obtained and the comparison between new and old values resumes. New layers will be added on until the SR value for each layer is between 1 and 1.2. The program then outputs the number of layers and the fibre angle of each layer. Figure 12 illustrates the procedure the script file follows to obtain the desired outputs. The FibreAngleOutput program was subjected to several runs. The ress, namely the number of layers and the fibre angles, needed to be verified. Therefore these were used as inputs in the Conventional Approach program. The TsaiWu failure theory was used and in each case there was no failure. As an eample, consider the graphite/epoy composite laminate eamined earlier. The material properties, material limits and loading conditions for this laminate were given in Table 1. The SR values for three layers with fibre angles of 0, 30 and 45 were shown in Figure 11. The values in Table 1
9 912 A. RAMSAROOP ET AL Obtain material properties and allowable limits Calculate [Q], [S] matrices Parameters for TsaiWu 5 4 Enter magnitude and angle of each force Resant forces and moments 6 Calculate all parameters: [T], [[Q Q ], h, z, z, A, A, B, B, D D midplane strains and curvatures global and local stresses and strains 12 Add new layer NO 11 Use TsaiWu failure criterion and find SR 10 Change angles YES Can SR be improved 9 NO 7 Use TsaiWu failure criterion and find SR 8 Is SR within acceptable limits YES 13 Output angles Figure 12. Flowchart describing the FibreAngleOutput program. were input into the FibreAngleOutput program. The output of the program is shown in Figure 13. It can be seen from Figure 13 that the number of layers is the same as when the eample was analysed by the Conventional Approach program; however, the fibre angles are different. Here the required angles are 49, 79 and 49 instead of the previous 0, 30 and 45. Further the SR values are all between 1 and 1.2 indicating no failure or overdesign. The new fibre angles (49, 79 and 49 ) along with the material properties, material limits and loading conditions in Table 1 were then input into the Conventional Approach program. The resing SR values were eactly the same as in Figure 13. Further, the local stresses of the new laminate, shown in Figure 14, was compared with the local stresses of the earlier laminate, shown in Figure 10. It can be seen that the local stresses in Figure 14 are constant through the thickness of each layer. This shows that the stresses were evenly distributed and not varied through the thickness of each layer. Previously the SR value on the first layer was less than 1 (Figure 11) and lower than the other two layers indicating earliest failure. However with the new layup, the SR value has increased to a value greater than one. This means that the first layer is now capable of carrying a higher load and this is evident by the values for the local stresses. The previous value at the top of the first layer was 33.5 MPa (Figure 10), and the new value is 75.7 MPa (Figure 14). This clearly demonstrates the higher load bearing capability of the new laminate. Similar trends may be seen from the other positions and from the other two layers.
10 A. RAMSAROOP ET AL. 913 Figure 13. Output of FibreAngleOutput program with Table 1 as input. Figure 14. Local stresses for laminate with angles of 49, 79, and 49. It was then decided to increase the loading conditions of the 49, 79 and 49 laminate to determine whether an increase in load will res in failure. The applied loads were increased by 10% and the resing SR values are shown in Figure 15. It can clearly be seen that all the SR values for all the layers were less than 1. An increase in loading resed in failure and therefore it may be deduced that the FibreAngleOutput program optimally designed the composite laminate for the loading conditions in Table 1. This further implies a saving in material cost as there would be no etra material used because of overdesigning.
11 914 A. RAMSAROOP ET AL. Figure 15. SR ratios for 49, 79 and 49 laminate with 10% increase in loading Finite Element Analysis For further verification of the computational ress, it was decided to perform finite element analyses on the laminates eamined in the Conventional Approach program and the FibreAngleOutput program. The package used for the analysis was MSC Patran/Nastran Two finite element models were setup, and both models represented a flat composite plate with material properties, material limits and loading conditions from Table 1. The first model had the same fibre layup that was used in the eample for the Conventional Approach program, that is, 0, 30, and 45. The analysis was run and the resing fringe plots of the stress components of each layer were plotted. These plots are shown in Figure 16. The stress plots from the finite element package corresponds to the local stresses eperienced by a laminate, in particular the stresses occurring at the middle of each layer. Comparing the stress values in Figure 16 with the stresses incurred at the middle of each layer in either Figure 6 or Figure 10, it can be seen that the values are eactly the same. This implies that the model was correctly setup and that it may be used to evaluate local stresses of laminates designed with the FibreAngle Output program. The second model was setup and was similar to the first model in every aspect ecept for the fibre layup. This model had the new fibre layup (49, 79, and 49 ) that was determined by the FibreAngleOutput program. The fringe plots of the stress components from this analysis are shown in Figure 17. Here it is also evident that the values in the plots eactly correspond to the stress values at the middle of each layer in Figure 14. This verifies the above ress from the FibreAngle Output program and supports the conclusion that the program optimally designed the composite laminate, with the fibre layup of 49, 79 and 49, for the loading conditions in Table Conclusions A MATLAB script file was generated that uses the conventional approach in the design of composite laminates. The inputs are the material properties, material limits, number of fibre layers, and the fibre orientation and thickness of each layer as well as the loading conditions. These values are then used in the governing equations, based on Hooke s law for twodimensional unidirectional laminates, to determine the global and local stresses and strains. The local stresses are compared to allowable limits via the TsaiWu failure theory. The ress from this program were compared to manually calculated eamples in the various tets [2,3] and it was found that they were eactly comparable. The above program required much guesswork in choosing inputs and was therefore inadequate to design composite laminates. Hence it was adapted to take material properties, material limits and the loading conditions as inputs. The necessary calculations were performed and the optimum number of fibre layers required as well
12 A. RAMSAROOP ET AL. 915 Figure 16. Fringe plots from Patran showing stress components for 0, 30, and 45 laminate. Figure 17. Fringe plots from Patran showing stress components for 49, 79, and 49 laminate.
13 916 A. RAMSAROOP ET AL. as the fibre angle of each layer was determined. These outputs were input into the Conventional Approach program in order to verify the ress. In each case the resing composite structure did not fail. The eample used showed that the FibreAngleOutput program optimally designed the composite laminate for the given loading conditions. Finite element analyses were conducted to verify this conclusion. The use of these programs will greatly reduce the design time of composite structures as the numerous computations are completed in a fraction of the time that it would take if done manually. The designer merely has to run the FibreAngleOutput program, and view the number of layers required and the fibre angle for each layer. The program will also aid in reducing material costs. Presently the program is limited to flat unidirectional structures but work is underway to etend it to three dimensions. There is no limit on the type of composite material as far as the matri and fibre reinforcement is concerned. 5. References [1] S. K. Mazumdar, Composite Manufacturing: Materials, Product, and Process Engineering, CRC Press LLC, Boca Raton, [2] A. K. Kaw, Mechanics of Composite Materials, CRC Press LLC, Boca Raton, [3] C. T. Herakovich, Mechanics of Fibrous Materials, John Wiley & Sons Inc., Hoboken, [4] R. M. Christensen, Mechanics of Composite Materials, Dover Publications, New York, [5] M. Akbulut and F. O. Sonmez, Optimum Design of Composite Laminates for Minimum Thickness, Computers and Structures, Vol. 86, No , 2008, pp [6] K. Sivakumar, N. G. R. Iyengar and K. Deb, Optimum Design of Laminated Composite Plates with Cutouts Using a Genetic Algorithm, Composite Structures, Vol. 42, No. 3, 1998, pp [7] S. A. Barakat and G. A. AbuFarsakh, The Use of an EnergyBased Criterion to Determine Optimum Configurations of Fibrous Composites, Composite Science and Technology, Vol. 59, No. 12, 1999, pp [8] P. Kere, M. Lyly and J. Koski, Using Micriterion Optimization for Strength Design of Composite Laminates, Composite Structures, Vol. 62, No. 34, 2003, pp [9] C. H. Park, W. I. Lee, W. S. Han and A. Vautrin, Weight Minimization of Composite Laminated Plates with Miple Constraints, Composite Science and Technology, Vol. 63, No. 7, 2003, pp [10] MediaWiki, MATLAB, wiki/matlab [11] R. V. Dukkipati, MATLAB for Mechanical Engineers, New Age International (P) Limited, New Delhi, [12] G. Z. Voyiadjis and P. I. Kattan, Mechanics of Composite Materials with MATLAB, Springer Netherlands, Dordrecht, [13] A. Gilat, MATLAB: An Introduction with Applications, John Wiley & Sons Inc., Hoboken, [14] B. D. Hahn and D. T. Valentine, Essential MATLAB for Engineers and Scientists, ButterworthHeinemann, Rome, 2007.
ON THE NUMERICAL ANALYSIS OF COMPOSITE MATERIAL
The 4th International Conference Advanced Composite Materials Engineering COMAT 8 October, Brasov, Romania O THE UMERICAL AALYSIS OF COMPOSITE MATERIAL D.D. icoara Transilvania University, City Brasov,
More informationModule 5: Laminate Theory Lecture 17: Laminate Constitutive Relations. The Lecture Contains: Laminate Constitutive Relations
Lecture 17: Laminate Constitutive Relations The Lecture Contains: Laminate Constitutive Relations Classification of Laminates CrossPly Laminates Specially Orthotropic Laminates Examples Homework References
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationComparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost
Comparison of Plywise StressStrain results for graphite/epoxy laminated plate subjected to inplane normal loads using CLT and ANSYS ACP PrepPost 1 Mihir A. Mehta, 2 Satyen D. Ramani 1 PG Student, Department
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationModule 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory. Introduction: The Lecture Contains: Laminate Theory with Thermal Effects
Module 5: Laminate Theory Lecture 19: Hygro thermal Laminate Theory Introduction: In this lecture we are going to develop the laminate theory with thermal and hygral effects. Then we will develop the
More informationPROMAL2012 SOFTWARE PACKAGE A USER GUIDE
PROMAL2012 SOFTWARE PACKAGE A USER GUIDE 1. This manual is only for VISTA, WINDOWS 7 and WINDOWS 8 users. The PROMAL2012 software and manual are available at http://www.eng.usf.edu/~kaw/promal2012/ 2.
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationME 7502 Lecture 2 Effective Properties of Particulate and Unidirectional Composites
ME 75 Lecture Effective Properties of Particulate and Unidirectional Composites Concepts from Elasticit Theor Statistical Homogeneit, Representative Volume Element, Composite Material Effective Stress
More informationComposites Design and Analysis. Stress Strain Relationship
Composites Design and Analysis Stress Strain Relationship Composite design and analysis Laminate Theory Manufacturing Methods Materials Composite Materials Design / Analysis Engineer Design Guidelines
More informationEffect of Thermal Stresses on the Failure Criteria of Fiber Composites
Effect of Thermal Stresses on the Failure Criteria of Fiber Composites Martin Leong * Institute of Mechanical Engineering Aalborg University, Aalborg, Denmark Bhavani V. Sankar Department of Mechanical
More informationStrength Prediction Of Composite Laminate
Strength Prediction Of Composite te Prof. Yogananda. A 1, Mr. R. Vijayakumar 2 Assistant Professor, Department of Mechanical Engineering, East West Institute of Technology, Bangalore. Research Scholar,
More informationAs an example we consider the stacking and analysis of a 2ply symmetric laminate. First we clear the Matlab space and close figures.
Program Lam 1 Introduction The collection of Matlab command and function files in the package lam allows the stacking and analysis of a laminate. In fact only a representative piece of a laminate is considered,
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More informationAmerican Society for Testing and Materials (ASTM) Standards. Mechanical Testing of Composites and their Constituents
Mechanical Testing of Composites and their Constituents American Society for Testing and Materials (ASTM) Standards Tests done to determine intrinsic material properties such as modulus and strength for
More informationCOMPUTER AIDED DESIGN IN CASE OF THE LAMINATED COMPOSITE MATERIALS
6 th International Conference Computational Mechanics and Virtual Engineering COMEC 15 1516 October 15, Braşov, Romania COMPUER AIDED DESIGN IN CASE OF HE LAMINAED COMPOSIE MAERIALS Camelia Cerbu ransilvania
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationSTRUCTURAL ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIALS CESAR AUGUSTO ROJAS. Presented to the Faculty of the Graduate School of
STRUCTURAL ANALYSIS OF FIBER REINFORCED COMPOSITE MATERIALS by CESAR AUGUSTO ROJAS Presented to the Faculty of the Graduate School of The University of Teas at Arlington in Partial Fulfillment of the Requirements
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of Materials Science and Engineering A 6 () 354 doi:.765/663/6..5 D DAVID PUBLISHING Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K * and V V Subba Rao Faculty
More informationMechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA What programs are in PROMAL? Master Menu The master menu screen with five separate applications from
More informationPLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
7th European Workshop on Structural Health Monitoring July 811, 2014. La Cité, Nantes, France More Info at Open Access Database www.ndt.net/?id=17206 PLY LEVEL UNCERTAINTY EFFECTS ON FAILURE OF COMPOSITE
More informationStress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina
Chapter 2 Macromechanical Analysis of a Lamina Stress, Strain Stress strain relationships for different types of materials Stress strain relationships for a unidirectional/bidirectional lamina Islamic
More informationOverview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling
Overview of Hygrothermally Stable Laminates with Improved Extensiontwist Coupling R. Haynes epartment of erospace Engineering, Georgia Institute of Technology 27 Ferst rive W, tlanta, G 33325, US robert.haynes@gatech.edu
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationCapability Assessment of Finite Element Software in Predicting the Last Ply Failure of Composite Laminates
Available online at www.sciencedirect.com Procedia Engineering 41 (2012 ) 1647 1653 International Symposium on Robotics and Intelligent Sensors 2012 (IRIS 2012) Capability Assessment of Finite Element
More informationPrediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach
Prediction of the Ultimate Strength of Composite Laminates Under InPlane Loading Prediction of The Ultimate Strength of Composite Laminates Under InPlane Loading Using A Probabilistic Approach Tae Jin
More informationAn integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale
An integrated approach to the design of high performance carbon fibre reinforced risers  from micro to macro  scale Angelos Mintzas 1, Steve Hatton 1, Sarinova Simandjuntak 2, Andrew Little 2, Zhongyi
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 34 Thermal Stresses in Plates Lecture Overview Introduction Mechanical and Thermal Strains
More informationINTERNATIONAL JOURNAL OF APPLIED ENGINEERING RESEARCH, DINDIGUL Volume 2, No 1, 2011
Interlaminar failure analysis of FRP cross ply laminate with elliptical cutout Venkateswara Rao.S 1, Sd. Abdul Kalam 1, Srilakshmi.S 1, Bala Krishna Murthy.V 2 1 Mechanical Engineering Department, P. V.
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationFinite Element Analysis of Graphite/Epoxy Composite Pressure Vessel
Journal of Materials Science and Chemical Engineering, 2017, 5, 1928 http://www.scirp.org/journal/msce ISSN Online: 23276053 ISSN Print: 23276045 Finite Element Analysis of Graphite/Epoxy Composite
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationA HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS
A HIGHERORDER BEAM THEORY FOR COMPOSITE BOX BEAMS A. Kroker, W. Becker TU Darmstadt, Department of Mechanical Engineering, Chair of Structural Mechanics Hochschulstr. 1, D64289 Darmstadt, Germany kroker@mechanik.tudarmstadt.de,
More informationNumerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure
Copyright c 007 ICCES ICCES, vol.1, no.3, pp.9398, 007 Numerical Analysis of Composite Panels in the PostBuckling Field taking into account Progressive Failure C. Bisagni 1 Summary The research here
More informationComposite Structures. Indian Institute of Technology Kanpur
Mechanics of Laminated Composite Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 23 Analysis of an Orthotropic Ply Lecture Overview Introduction Engineering constants for an 2
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More information15 INTERLAMINAR STRESSES
15 INTERLAMINAR STRESSES 151 OUTOFPLANE STRESSES Classical laminate plate theor predicts the stresses in the plane of the lamina,, and τ but does not account for outofplane stresses, τ and τ. It assumes
More informationFailure analysis of serial pinned joints in composite materials
Indian Journal of Engineering & Materials Sciences Vol. 18, April 2011, pp. 102110 Failure analysis of serial pinned joints in composite materials Alaattin Aktaş* Department of Mechanical Engineering,
More informationA RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION
A RESEARCH ON NONLINEAR STABILITY AND FAILURE OF THIN WALLED COMPOSITE COLUMNS WITH OPEN CROSSSECTION H. Debski a*, J. Bienias b, P. Jakubczak b a Faculty of Mechanical Engineering, Department of Machine
More information46th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference April 2005 Austin, Texas
th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference  April, Austin, Texas AIAA  AIAA  Bistable Cylindrical Space Frames H Ye and S Pellegrino University of Cambridge, Cambridge,
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More information1.105 Solid Mechanics Laboratory Fall 2003
1.105 Solid Mechanics Laboratory Fall 2003 Eperiment 6 The linear, elastic behavior of a Beam The objectives of this eperiment are To eperimentally study the linear elastic behavior of beams under four
More informationLAMINATED COMPOSITE PLATES
LAMINATED COMPOSITE PLATES David Roylance Department of Materials Science and Engineering Massachusetts Institute of Technology Cambridge, MA 02139 February 10, 2000 Introduction This document is intended
More informationOnline publication date: 23 October 2010
This article was downloaded by: [informa internal users] On: 1 November 2010 Access details: Access Details: [subscription number 755239602] Publisher Taylor & Francis Informa Ltd Registered in England
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationModule 7: Micromechanics Lecture 29: Background of Concentric Cylinder Assemblage Model. Introduction. The Lecture Contains
Introduction In this lecture we are going to introduce a new micromechanics model to determine the fibrous composite effective properties in terms of properties of its individual phases. In this model
More informationMINE ROOF SUPPORT DESIGN AND ANALYSIS. Document no : Revision no : 1.0
MINE ROOF SUPPORT DESIGN AND ANALYSIS Document no : 1806269723 Revision no : 1.0 DOCUMENT TITLE : MINE ROOF SUPPORT DESIGN AND ANALYSIS DOCUMENT NUMBER : 1806269723 ISSUE : Issue 1.0 DATE : 7 October
More informationThe stiffness of plates
The stiffness of plates 1. Introduction The word plate is a collective term for elements in which forces can be transferred in two directions. Floors, walls, bridge slabs and laminates are all plates.
More informationA Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber
A Study on the Tube of Integral Propeller Shaft for the Rearwheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmuro, Goesangun, South Korea.
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationComposite Laminate Modeling
omposite Laminate Modeling White Paper for Femap and NX Nastran Users Venkata Bheemreddy, Ph.D., Senior Staff Mechanical Engineer Adrian Jensen, PE, Senior Staff Mechanical Engineer WHAT THIS WHITE PAPER
More information8 Properties of Lamina
8 Properties of Lamina 8 ORTHOTROPIC LAMINA An orthotropic lamina is a sheet with unique and predictable properties and consists of an assemblage of fibers ling in the plane of the sheet and held in place
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationStacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous Orthotropic Laminates.
49th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials 710 April 2008, Schaumburg, IL AIAA 20081940 Stacking sequences for Extensionally Isotropic, Fully Isotropic and QuasiHomogeneous
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationMECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING
MECHANICAL FAILURE OF A COMPOSITE HELICOPTER STRUCTURE UNDER STATIC LOADING Steven Roy, Larry Lessard Dept. of Mechanical Engineering, McGill University, Montreal, Québec, Canada ABSTRACT The design and
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationDesign and Analysis of a Formula Student Carbon Fibre Rim
THE 5 th STUDENT SYMPOSIUM ON MECHANICAL AND MANUFACTURING ENGINEERING Design and Analysis of a Formula Student Carbon Fibre Rim K. Korntved, J. Hersbøll, M. Lauritsen, K. Bording, H. Leto Department of
More informationSmart Materials, Adaptive Structures, and Intelligent Mechanical Systems
Smart Materials, Adaptive Structures, and Intelligent Mechanical Systems Bishakh Bhattacharya & Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 19 Analysis of an Orthotropic Ply References
More informationOutline. Organization. Stresses in Beams
Stresses in Beams B the end of this lesson, ou should be able to: Calculate the maimum stress in a beam undergoing a bending moment 1 Outline Curvature Normal Strain Normal Stress Neutral is Moment of
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationACDC. User Manual. Ver. 1.0
ACDC User Manual Ver. 1.0 Centre Composite December 2016 ACDC, Ver. 1.0 User Manual Centre Composite, 2016 (software@composite.lv) Table of Contents Introduction... 1 System requirements... 1 Theoretical
More informationFinite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix)
Finite Element Analysis of Composite Laminate By Using ABDH Matrix(Stiffness Matrix) Nikhil J. Chaudhari 1 Post Graduate Student Department of Mechanical Engineering Veermata Jijabai Technological Institute
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationPassive Damping Characteristics of Carbon Epoxy Composite Plates
Journal of aterials Science and Engineering A 6 (12) (2016) 3542 doi: 10.17265/21616213/2016.12.005 D DAVID PUBLISHIG Passive Damping Characteristics of Carbon Epoxy Composite Plates Dileep Kumar K
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationMAAE 2202 A. Come to the PASS workshop with your mock exam complete. During the workshop you can work with other students to review your work.
It is most beneficial to you to write this mock final exam UNDER EXAM CONDITIONS. This means: Complete the exam in 3 hours. Work on your own. Keep your textbook closed. Attempt every question. After the
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More informationFinite element analysis of drilled holes in unidirectional composite laminates using failure theories
American Journal of Science and Technology 2014; 1(3): 101105 Published online May 30, 2014 (http://www.aascit.org/journal/ajst) Finite element analysis of drilled holes in unidirectional composite laminates
More informationMechanics Of Composite Materials (Dover Civil And Mechanical Engineering) By Richard M. Christensen, Engineering READ ONLINE
Mechanics Of Composite Materials (Dover Civil And Mechanical Engineering) By Richard M. Christensen, Engineering READ ONLINE The impact of fiber loading and length on mechanical properties like tensile
More informationCOMPARISON OF PLATE MODELS FOR ANALYSIS OF LAMINATED COMPOSITES
COMPARISON OF PLATE MODELS FOR ANALYSIS OF LAMINATED COMPOSITES P. M. Mohite and C. S. Upadhyay** Department of Aerospace Engineering, IIT Kanpur 0806, INDIA, email: mohite@iitk.ac.in Assistant Professor,
More informationModule 7: Micromechanics Lecture 34: Self Consistent, Mori Tanaka and Halpin Tsai Models. Introduction. The Lecture Contains. Self Consistent Method
Introduction In this lecture we will introduce some more micromechanical methods to predict the effective properties of the composite. Here we will introduce expressions for the effective properties without
More informationDevelopment of a code to generate randomly distributed short fiber composites to estimate mechanical properties using FEM
International Journal of Theoretical and Applied Mechanics. ISSN 09736085 Volume 12, Number 4 (2017) pp. 863872 Research India Publications http://www.ripublication.com Development of a code to generate
More informationComposite models 30 and 131: Ply types 0 and 8 calibration
Model calibration Composite BiPhase models 30 and 3 for elastic, damage and failure PAMCRASH material model 30 is for solid and 3 for multilayered shell elements. Within these models different ply types
More informationDynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load
Dynamic Analysis of Laminated Composite Plate Structure with Square CutOut under Hygrothermal Load Arun Mukherjee 1, Dr. Sreyashi Das (nee Pal) 2 and Dr. A. Guha Niyogi 3 1 PG student, 2 Asst. Professor,
More informationBISTABLE COMPOSITE SHELLS
AIAA 21385 BISTABLE COMPOSITE SHELLS K. Iqbal and S. Pellegrino Department of Engineering, University of Cambridge, Trumpington Street, Cambridge, CB2 1PZ, U.K. Abstract This paper is concerned with
More informationFailure Analysis of Unidirectional Composite Pinned Joints
217 IJEDR Volume, Issue 4 ISSN: 23219939 Failure Analysis of Unidirectional Composite Pinned Joints 1 Sai Ashok.M, 2 Mr. U. Koteswara Rao 1 Mtech Machine Design, 2 Associate Professor & Asst. COE 1
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 20, 2011 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 20, 2011 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS LAST NAME (printed): FIRST NAME (printed): STUDENT
More informationFig. 1. Circular fiber and interphase between the fiber and the matrix.
Finite element unit cell model based on ABAQUS for fiber reinforced composites Tian Tang Composites Manufacturing & Simulation Center, Purdue University West Lafayette, IN 47906 1. Problem Statement In
More informationNUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE
Journal of KONES Powertrain and Transport, Vol. 19, No. 1 2012 NUMERICAL FEM ANALYSIS FOR THE PART OF COMPOSITE HELICOPTER ROTOR BLADE Hubert D bski Lublin University of Technology, Department of Machine
More informationModule6: Laminated CompositesII. Learning Unit1: M6.1. M 6.1 Structural Mechanics of Laminates
Module6: Laminated CompositesII Learning Unit1: M6.1 M 6.1 Structural Mechanics of Laminates Classical Lamination Theory: Laminate Stiffness Matrix To this point in the development of classical lamination
More informationMost of the material in this package is based on a recently published book. This is:
Mechanics of Composite Materials Version 2.1 Bill Clyne, University of Cambridge Boban Tanovic, MATTER Assumed Preknowledge It is assumed that the student is familiar with simple concepts of mechanical
More informationProbabilistic Failure Analysis of Composite Beams for Optimum Ply Arrangements under Ballistic Impact
Journal of Aerospace Science and Technology 1 (015) 3647 doi: 10.1765/33858/015.01.005 D DAVID PUBLISHING Probabilistic Failure Analysis of Composite Beams for Optimum Ply Shivdayal Patel, Suhail Ahmad
More informationA Stress Gradient Failure Theory for Textile Structural Composites. Final Technical Report submitted to ARO
A Stress Gradient Failure Theory for Textile Structural Composites Final Technical Report submitted to ARO By RYAN KARKKAINEN and BHAVANI SANKAR University of Florida Department of Mechanical & Aerospace
More informationEXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS
EXPLICIT DYNAMIC SIMULATION OF DROPWEIGHT LOW VELOCITY IMPACT ON CARBON FIBROUS COMPOSITE PANELS Umar Farooq and Karl Gregory School of Built Environment and Department of Engineering, University of Bolton,
More informationDYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES
Association of Metallurgical Engineers of Serbia AMES Scientific paper UDC:669.1419:628.183=20 DYNAMIC FAILURE ANALYSIS OF LAMINATED COMPOSITE PLATES J. ESKANDARI JAM 1 and N. GARSHASBI NIA 2 1 Aerospace
More informationME 323 Examination #2 April 11, 2018
ME 2 Eamination #2 April, 2 PROBLEM NO. 25 points ma. A thinwalled pressure vessel is fabricated b welding together two, openended stainlesssteel vessels along a 6 weld line. The welded vessel has an
More informationAERSYS KNOWLEDGE UNIT
7016 1. INTRODUCTION The scope of this document is to provide a clarification and a deeper understanding of the two different ways to move the mid plane of the element out of the nodal plane. Although
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationLongitudinal buckling of slender pressurised tubes
Fluid Structure Interaction VII 133 Longitudinal buckling of slender pressurised tubes S. Syngellakis Wesse Institute of Technology, UK Abstract This paper is concerned with Euler buckling of long slender
More information